Reduced activation ferritic/martensitic sently considered as the primary candidatefuture fusion reactors based upon their lowgood resistance to void swelling, good thand relatively mature material fabricationThe structural materials for future fusion
e ux oon can
of its properties tested before irradiations are similar to those ofthe other RAFMs under wide research in the world [1,610]. AndCLAM is chosen as the candidate structure material of the FDS ser-ies fusion reactors  and ITER liquid LiPb Test Blanket Mod-ule of China . To investigate the irradiation effects onCLAM, neutron irradiation experiments are being carried out underwide collaboration in China and overseas.
In this paper, the low dose neutron irradiation experiment onCLAM specimens to 0.02 dpa at 250 C was introduced. The effects
Specimens of CLAM were irradiated in a ssion reactor to0.02 dpa at 250 C. Tensile tests using 51 mm length specimenswith a gage part of U4 20 mm were carried out at room temper-ature (RT), 150 C, 200 C and 300 C in a static tensile machine at across-head speed of 0.1 mm/min before yield point and 5 mm/minafter yield point. The lower deformation rate before yield point wasto investigate the elastic deformation of specimens. Charpy impacttests using specimens (55 10 10 mm) with a 45 2 mmV-notch were performed in the test temperature range from120 C to 60 C.
* Corresponding author.
Journal of Nuclear Materials 386388 (2009) 312314
Contents lists availab
lsE-mail address: email@example.com (L. Peng).material were widely carried out to investigate the irradiation ef-fects. The effects of irradiation on the mechanical properties de-pend on irradiation temperature; for irradiations above 400 C,properties are generally unchanged, although the occurrence ofradiation-enhanced softening has been reported. Changes inmechanical properties tend to saturate with increasing dose; forsome RAFM steels, saturation has been observed around 10 dpa .
Research on a new version of RAFMs i.e. China Low ActivationMartensitic steel (CLAM) was started ve years ago at ASIPP (Insti-tute of Plasma Physics, Chinese Academy of Sciences) under widecollaboration with other institutes and universities in China. Most
Table 1. HEAT 0408B and HEAT 0603A are the alloy with normalcomposition design and 0.3% silicon was added in HEAT 0408Dto investigate the effect of silicon on the mechanical property.
The specimens of HEAT 0408B and HEAT 0408D were from20 kg ingot, which was hot-forged and rolled into a 6 mm-thickplate and 12 mm-thick plate. The specimens of HEAT 0603A werefrom 300 kg ingot, which was hot-forged and rolled into a12.5 mm-thick plate. The heat treatments included normalization(980 C/30 min/air cool) and tempering (760 C/90 min/air cool).The details of metallurgical process and composition for themcan be found in Refs. [1,7].high displacement damage by intensSo neutron irradiation experiments0022-3115/$ - see front matter Crown Copyright 2doi:10.1016/j.jnucmat.2008.12.119teels (RAFMs) are pres-structural material forresidual radioactivity,
ermal stress resistancetechnologies etc. .reactors will undergof high energy neutrons.didate fusion structural
of low dose neutron irradiation on mechanical properties of CLAMwere analyzed. Besides, irradiation effects on CLAM and other RAF-Ms under similar irradiation conditions were introduced andcompared.
The steels used were HEAT 0408B, HEAT 0408D and HEAT0603A of CLAM. Their chemical compositions are listed inPreliminary analysis of irradiation effectsneutron irradiation
Lei Peng a,*, Qunying Huang a,b, Chunjing Li a, Shaojua Institute of Plasma Physics, Chinese Academy of Sciences, Hefei, Anhui 230031, Chinab School of Nuclear Science and Technology, University of Science and Technology of Chi
a r t i c l e i n f o a b s t r a c t
To investigate the irradiat(RAFMs) i.e. China Low Acbeing carried out under wities of CLAM heats 0603A,0.02 dpa at 250 C. The0603A increased about 105 C. For CLAM heats 0408
Journal of Nu
journal homepage: www.e009 Published by Elsevier B.V. Alln CLAM after low dose
efei, Anhui 230027, China
effects on a new version of reduced activation ferritic/martensitic steelstion Martensitic steel (CLAM), neutron irradiation experiments has beencollaboration in China and overseas. In this paper, the mechanical proper-8B, and 0408D were investigated before and after neutron irradiation toresults showed that ultimate strength and yield stress of CLAM HEATMPa and ductile to brittle transition temperature (DBTT) shift was aboutd 0408D, ultimate strength and yield stress increased about 80150 MPa.Crown Copyright 2009 Published by Elsevier B.V. All rights reserved.
le at ScienceDirect
evier .com/locate / jnucmatrights reserved.
3. Results and discussion
3.1. Tensile properties
Fig. 1 shows the strength and elongation for HEAT 0603A beforeand after irradiation. The ultimate strength and yield stress in-creased about 1030 MPa. Total elongation decreased about 4% at200 C and 350 C but increased about 4% at RT and 100 C. Andthe reduction of area decreased 14% at different temperatures.
It was reported that the increase of strength of 9Cr2WVTa after0.015 dpa neutron irradiation at 60100 C was 30 MPa and totalelongation decreased about 6% . So hardening of CLAM wasslight, after low dose neutron irradiation.
Fig. 2 shows the strength and elongation for HEAT 0408B beforeand after irradiation. The ultimate strength increased about 80120 MPa and yield stress increased about 100150 MPa. Total
elongation decreased about 6% at RT. The specimens before irradi-ation are 6 mm-thick plate.
Fig. 3 shows the strength and elongation for HEAT 0408D beforeand after irradiation. The ultimate strength increased about100 MPa and yield stress increased about 80150 MPa. Total elon-gation decreased about 8%. The specimens before irradiation are6 mm-thick plate.
For the tensile results of HEAT 0408B and HEAT 0408D, there isno obvious silicon effect on the irradiation hardening. Irradiationinduced hardening of HEAT 0408B and HEAT 0408D are much lar-ger than that of HEAT 0603A. To determine the source of thesemuch higher hardening levels, detailed microstructural character-ization investigation is underway.
3.2. Impact properties
Fig. 4 shows the charpy impact curves for HEAT 0603A beforeand after irradiation, tted with hyperbolic tangent function. Theductile-brittle transition temperature (DBTT), obtained at the tem-perature corresponding to half the difference between the upper-shelf energy and lower-shelf energy, increased about 5 C afterirradiation.
It was reported that the DBTT shift of JLF-1 after 0.01 dpa neu-tron irradiation at 297 C was 50 C . The embrittlement of
Table 1Chemical compositions of different heats of CLAM steel (wt%).
Cr W V Ta Mn C Si
HEAT 0408B 8.91 1.44 0.20 0.15 0.49 0.12 0.11HEAT 0408D 8.91 1.44 0.20 0.15 0.49 0.12 0.27HEAT 0603A 8.93 1.44 0.20 0.15 0.45 0.13 0.08
L. Peng et al. / Journal of Nuclear Materials 386388 (2009) 312314 313Fig. 1. Tensile propertiFig. 2. Tensile properties of CLAM (HEAT 0603A).f CLAM (HEAT 0408B).
314 L. Peng et al. / Journal of Nuclear Materials 386388 (2009) 312314Fig. 3. Tensile propertiCLAM was slighter compared with that of JLF-1 after low dose neu-tron irradiation.
Tensile specimens of HEAT 0408B, HEAT 0408D and HEAT0603A and Charpy specimens of HEAT 0603A were irradiated at250 C to 0.02 dpa. Hardening and embrittlement of CLAM oc-curred after irradiation:
(1) The ultimate strength and yield stress of HEAT 0603Aincreased 1030 MPa and total elongation decreased about4%.
Fig. 4. Charpy impact curves of CLAM (HEAT 0603A).(2) The DBTT shift of CLAM HEAT 0603A, obtained at half thedifference between the upper-shelf energy and lower-shelfenergy, is about 5 C.
(3) For CLAM heats 0408B and 0408D, ultimate strength andyield stress increased about 80150 MPa.
This work was supported by the National Natural Science Foun-dation of China with the Grant Nos. 10775135 and 10675123, theJSPS-CAS Core University Program and the National Basic ResearchProgram of China with the Grant No. 2008cb717802.
 Q. Huang, C. Li, Y. Li, et al., J. Nucl. Mater. 367370 (2007) 142. B. van der Schaaf, D.S. Gelles, S. Jitsukawa, et al., J. Nucl. Mater. 283287 (2000)
52. R.L. Klueh, D.S. Gelles, S. Jitsukawa, et al., J. Nucl. Mater. 307311 (2002) 455. T. Muroga, M. Gasparotto, S.J. Zinkle, et al., Fus. Eng. Des. 61&62 (2002) 13. E. Lucon, P. Benoit, P. Jacquet, et al., Fus. Eng. Des. 81 (2006) 917. Q. Huang, J. Li, Y. Chen, J. Nucl. Mater. 329333 (2004) 268. Y. Li, Q. Huang, Y. Wu, et al., J. Nucl. Mater. 367370 (2007) 117.
f CLAM (HEAT 0408D). C. Li, Q. Huang, P. Zhang, et al., Fus. Eng. Des. 82 (2007) 2627. Y. Li, Q. Huang, Y. Wu, et al., Fus. Eng. Des. 82 (2007) 2683. C. Li, Q. Huang, Y. Feng, et al., Plasma Sci. Technol. 9 (4) (2007) 484. Y. Wu, S. Zheng, X. Zhu, et al., J. Nucl. Mater. 307311 (2002) 1629. Y. Wu, FDS Team, Fus. Eng. Des. 83 (2008) 1683. Y. Wu, FDS Team, J. Nucl. Mater. 386388 (2009) 122. Y. Wu, W. Wang, S. Liu, et al., Chin. J. Nucl. Sci. Eng. 25 (4) (2005) 347. Y. Wu, FDS Team, Nucl. Fusion 47 (2007) 1. Y. Wu, Fusion Eng. Des. 82 (2007) 1893. K. Farrell, J. Nucl. Mater. 318 (2003) 274. Y. Kohno, A. Kohyama, T. Hirose, J. Nucl. Mater. 271&272 (1999) 145.
Preliminary analysis of irradiation effects on CLAM after low dose neutron irradiationIntroductionExperimentalResults and discussionTensile propertiesImpact properties